Semiconductor Quantum Dots and Quantum Dot lawm/Semiconductor quantum dots and quantum...
Embed Size (px)
Transcript of Semiconductor Quantum Dots and Quantum Dot lawm/Semiconductor quantum dots and quantum...
Semiconductor Quantum Dots and Quantum Dot Arrays and Applications ofMultiple Exciton Generation to Third-Generation Photovoltaic Solar Cells
A. J. Nozik,*,, M. C. Beard, J. M. Luther, M. Law, R. J. Ellingson,| and J. C. Johnson
The National Renewable Energy Laboratory, 1617 Cole Boulevard, Golden, Colorado 80401, United States, Department of Chemistry andBiochemistry, University of Colorado, Boulder, Colorado 80309, United States, Department of Chemistry, University of California, Irvine, Irvine,
California 92697, United States, and Department of Physics and Astronomy, University of Toledo, Toledo, Ohio 43606, United States
Received August 25, 2009
1. Introduction 68732. Synthesis of Colloidal Quantum Dots 6874
2.1. Solution Synthesis 68742.2. III-V Quantum Dots Grown via Vapor Phase
3. Relaxation Dynamics of Photogenerated CarriersIn QDs
3.1. Experimental Determination of Relaxation/Cooling Dynamics and a Phonon Bottleneck inQuantum Dots
4. Multiple Exciton Generation (MEG) in QuantumDots
4.1. MEG in Si QDs 68805. Quantum Dot Arrays 6881
5.1. MEG in PbSe QD Arrays 68826. Applications: Quantum Dot Solar Cells 6884
6.1. Quantum Dot Solar Cell Configurations 68856.1.1. Photoelectrodes Composed of Quantum
6.1.2. Quantum Dot-Sensitized NanocrystallineTiO2 Solar Cells
6.1.3. Quantum Dots Dispersed in OrganicSemiconductor Polymer Matrices
6.2. Schottky Junction and p-n Junction SolarCells Based on Films of QD Arrays
7. Conclusion 68878. Acknowledgments 68879. Note Added after ASAP Publication 6887
10. References 6887
1. IntroductionSemiconductors show dramatic quantization effects when
charge carriers (electrons and holes) are confined by potentialbarriers to small regions of space where the dimensions of theconfinement are less than the de Broglie wavelength of thecharge carriers, or equivalently, the nanocrystal diameter is lessthan twice the Bohr radius of excitons in the bulk material. Thelength scale at which these effects begin to occur in semicon-ductors is less than about 25 to 10 nm depending upon effectivemasses. When the charge carriers are confined by potential
barriers in three spatial dimensions, this regime is termed aquantum dot (QD). Two-dimensional confinement producesquantum wires or rods, while one-dimensional confinementproduces quantum films. QDs can be formed either by epitaxialgrowth from the vapor phase (molecular beam epitaxy (MBE)or metallo-organic chemical vapor deposition (MOCVD) pro-cesses) or via chemical synthesis (colloidal chemistry orelectrochemistry). QDs are also frequently referred to asnanocrystals (NCs). However, the term nanocrystal covers arange of shapes other than spherical in the nanoscale, such asnanowires, nanorods, nanotubes and nanoribbons,1-7 nano-rings,8-11 and nanotetrapods.12-14 The nanocrystals referred tohere are semiconductor particles quantum confined in threedimensions.
The use of semiconductor nanocrystals that exhibit quan-tization effects in solar photoconversion devices (mainlyquantum dots, quantum wires, and quantum rods) is presentlyattracting a great level of interest.15-23 Such QD-baseddevices used as photovoltaic cells are now labeled third-generation or next-generation PV24,25 because new advancesin the photophysics allows for the possibility of theseinexpensive materials to be incorporated into device struc-tures with potential efficiency much higher than the ther-modynamic limit for single junction bulk solar cells. Theconcept of the use of quantization effects in semiconductorsto enhance solar photoconversion performance that nowforms the basis for much of what is now known as third-generation solar conversion originated in the late 1970s andearly 1980s, with the concept of hot electron utilization andits enhancement through quantum confinement in varioussemiconductor nanostructures.26-30
Beginning in the early 1980s, quantum dots of groupsII-VI, III-V, IV-VI, and IV were specifically synthesizedto investigate size quantization effects; prior to this period,nanocrystals had been utilized in various materials to achievecertain effects through empirical exploration such as colorcontrol in stained glass, but their quantized nature was notrecognized until the 1970s. This early work has beenreviewed by several authors.31-40 CdS, CdSe, CdTe, InP,GaAs, GaP, GaN, GaInP, core-shell InP/ZnCdSe2, Ge, andSi QDs were among the early reported syntheses.31-38
Beginning in the 1990s and extending to today, thesyntheses of NCs and QDs have improved greatly; theseadvances include lower reaction temperatures, one-potsyntheses, better size control and size dispersion, newmaterials systems, better shape control, heterostructuredparticles such as core-shell QDs or end-on attachment, andbetter control and understanding of surface chemistry. These
* To whom correspondence should be addressed. E-mail: [email protected] The National Renewable Energy Laboratory. University of Colorado. University of California, Irvine.| University of Toledo.
Chem. Rev. 2010, 110, 68736890 6873
10.1021/cr900289f 2010 American Chemical SocietyPublished on Web 10/14/2010
advances have been described in several recent reviews andpapers31,41-54 and will not be reviewed here. Reviews of workon nanowires, rods, rings, tubes, ribbons, and tetrapods areavailable.1-10,12-14,55
Here, we will first briefly summarize the general principles ofQD synthesis using our previous work on InP as an example. Thenwe will focus on QDs of the IV-VI Pb chalcogenides (PbSe, PbS,and PbTe) and Si QDs because these were among the first QDsthat were reported to produce multiple excitons upon absorbingsingle photons of appropriate energy (a process we call multipleexciton generation (MEG)). We note that in addition to Si and thePb-VI QDs, two other semiconductor systems (III-V InP QDs56and II-VI core-shell CdTe/CdSe QDs57) were very recentlyreported to also produce MEG. Then we will discuss
photogenerated carrier dynamics in QDs, including the issuesand controversies related to the cooling of hot carriers andthe magnitude and significance of MEG in QDs. Finally, wewill discuss applications of QDs and QD arrays in novelquantum dot PV cells, where multiple exciton generationfrom single photons could yield significantly higher PVconversion efficiencies.
2. Synthesis of Colloidal Quantum Dots
2.1. Solution SynthesisThe most common approach to the synthesis of colloidal
ionic QDs is the controlled nucleation and growth of particlesin a solution of chemical precursors containing the metaland the anion sources (controlled arrested precipitation).48,58-60
The technique of forming monodispersed colloids is veryold and can be traced back to the synthesis of gold colloids
Dr. Arthur J. Nozik is a Senior Research Fellow at the U.S. DOE NationalRenewable Energy Laboratory (NREL), Professor Adjoint in the Departmentof Chemistry and Biochemistry at the University of Colorado, Boulder,and a Fellow of the NREL/University of Colorado Renewable andSustainable Energy Institute. In 2009, Nozik was selected as AssociateDirector of a joint Los Alamos National Lab/NREL Energy FrontierResearch Center for DOE called Center for Advanced Solar Photophysics.Between 2006 and 2009 he served as the Scientific Director of the Centerfor Revolutionary Solar Photoconversion under the Colorado RenewableEnergy Collaboratory. Nozik received his BChE from Cornell Universityin 1959 and his Ph.D. in Physical Chemistry from Yale University in 1967.Before joining NREL in 1978, then known as the Solar Energy ResearchInstitute (SERI), he conducted research at the Materials Research Centerof the Allied Chemical Corporation (now Honeywell, Inc.). Dr. Noziksresearch interests include size quantization effects in semiconductorquantum dots and quantum wells, including multiple exciton generationfrom a single photon; the applications of unique effects in nanostructuresto advanced approaches for solar photon conversion; photogeneratedcarrier relaxation dynamics in various semiconductor structures; photo-electrochemistry of semiconductor-molecule interfaces; photoelectro-chemical energy conversion; photocatalysis; optical, magnetic, andelectrical properties of solids; and Mossbauer spectroscopy. He haspublished over 250 papers and book chapters in these fields, written oredited five books, holds 11 U.S. patents, and has delivered over 275invited talks at universities, conferences, and symposia. He has servedon numerous scientific review and advisory panels, chaired and organizedmany international and national conferences, workshops, and symposia,and received several awards in solar energy research, including the 2009Science and Technology Award from the Intergovernmental RenewableEnergy Organization associated with the United Nations, the 2008 EniAward from the President of Italy, and the 2002 Research Award of theElectrochemical Society. Dr. Nozik has been a Senior Editor of The Journalof Physical Chemistry from 1993 to 2005 and is on the editorial advisoryboard of the Journal of Energy and Environmental Sciences and theJournal of Solar Energy Materials and Solar Cells. A Special FestschriftIssue of the Journal of Physical Chemistry honoring Dr. Noziks scientificcareer appeared in the December 21, 2006 issue. Dr. Nozik is a Fellowof the American Physical Society and a Fellow of the American Associationfor the Advancement of Science; he is also a member of the AmericanChemical Society, the Electrochemical Society, and the Materials ResearchSociety.
Matthew C. Beard is a Senior Scientist at the National Renewable EnergyLaboratory. He received his B.Sc. And M.Sc. Degrees in Chemistry fromBrigham Young University in 1997 and Ph.